Homoepitaxial growth of alumina
films on NiAl(110) using NO
submitted in partial fulfillment of the requirements for the degree of
BACHELOR OF SCIENCE
Author : Joost Vermeer
Student ID :
Supervisor : Irene Groot
Homoepitaxial growth of alumina
films on NiAl(110) using NO
Huygens-Kamerlingh Onnes Laboratory, Leiden University P.O. Box 9500, 2300 RA Leiden, The Netherlands
January 17, 2019
In the search for substrates used in the investigation of catalytic nanoparticles we have grown alumina films on NiAl(110) past
5.35 ˚A, the maximum thickness that can be obtained with molecular oxygen . A NiAl(110) sample was first oxidized to that thickness with molecular oxygen, after which it was stepwise
oxidized with NO2. The film thickness, crystal structure and
chemical composition were measured using Low Energy Electron Diffraction (LEED), X-ray Photoelectron Spectroscopy (XPS) and Scanning Tunneling Microscopy (STM). We have confirmed that film grown with NO2follows the theoretical model of Cabrera
and Mott up to 6.9 ˚A. STM images show an increase in the number of islands and vacancies in the metal, indicating that this
1 Introduction 1
2 Theory 5
2.1 Quantitative description of oxide film growth 5 2.2 Qualitative description of oxide film growth 7
3 Experimental Methods 11
3.1 Equipment 11
3.2 General Approach 12
3.3 Sample preparation 13
3.4 XPS Fitting 15
3.5 XPS measurement of film thickness 16
4 Results and discussion 21
4.1 Crystal structure 21
4.2 Film thickness 23
4.3 Film growth location 25
4.4 Stability of MoO3nanoparticles 26
4.5 Carbon contamination 27
In their attempt to find ever better catalysts, chemical companies have turned to nanoparticles. These particles have many properties that their bulk states do not have, like special facets and a high surface to mass ratio. To use them in an industrial setting they need to be placed on a support, or they would be carried away by the flow of the the gas or liquid it is re-acting with. One of the most common used supports is aluminum oxide, also called alumina. It is strong, cheap and chemically inert, which makes it ideal in situations where one does not want any uncontrolled reactions happening.
Our group investigate these industrial catalytic processes. We try to mimic the industrial circumstances as close as possible, but unfortunately that is not possible in this case. Bulk alumina is hard to investigate in an academic setting since research groups cannot use one of their most important measurement methods, Scanning Tunneling Microscopy (STM). An STM setup consists of a conducting tip which is about a nanometer away from the surface. If the surface is conducting, a voltage difference between the tip and the sample creates a tunneling current. This tunneling current is measurable and depends on both the distance between the tip and the sample, as well as the electronic state of the surface. But if the sample is an electrical insulator this is impossible, since there is no low potential area for the electrons to tunnel to.
crystal structure. The film has a limited growth in molecular oxygen, since the energy for oxygen adsorption comes from electrons tunneling from the metal to the film surface. In thicker films the tunneling current decreases which lowers the energy available at the surface. At a certain point adsorp-tion is no longer thermodynamically favored and the film stops growing.
Molybdenum oxide nanoparticles
A system that was previously studied by our group was MoO3
nanopar-ticles on an O2limited alumina film  and their catalytic behavior in the
desulfurization of sulfur-containing hydrocarbons. When investigating the MoO3 nanoparticles it was discovered that the molybdenum was
re-duced to metal and the alumina film thickness was increasing. This could only be explained by assuming that the MoO3dissociates, with the oxygen
atoms moving into the alumina film, increasing its thickness.
In order to further investigate this system we need to prevent the ciation of the molybdenum oxide. Since the energy required for the disso-ciation originates from the electrons tunneling through the metal, and the tunneling current depends on the thickness of the film barrier, a thicker film will reduce the energy available for dissociation. If the film is thick enough, the amount of energy available at the surface will be so low that the oxygen atoms remain within the molybdenum oxide. At such a thick-ness the molybdenum oxide and the desulfurization of sulfur-containing hydrocarbons can be investigated as if we were investigating the bulk alu-mina.
There is one important condition for this to work. We still have to be able to scan the surface with STM. Since the alumina is an insulator the electrons have to tunnel through the film as well. The thicker the film is, the larger the distance between the tip and the NiAl support. This de-creases the tunneling current and lowers the signal to noise ratio. To pre-vent that we could move closer the tip is to the alumina surface, but doing so would increase the probability that the tip crashes into the sample. It is therefore questionable whether we are able to scan on the thick films and actually investigate the nanoparticles.
There is more unknown about this plan. It is unclear which properties of the O2 limited alumina film remain past the O2 limit. Therefore these
properties, especially the crystal structure and growth speed, need to be investigated at thicker films. It also gives us opportunities. Since the O2
limited film is quite stable, unlike the thinner films, we should be able to answer one of the open questions of Cabrera-Mott growth : Where does
the film grow? This is an interesting question in itself, which we are able to investigate in this project.
In order to answer all those questions we will stepwise increase the film thickness with NO2 while investigating the surface in between, up
to the point where STM becomes almost impossible. At that point MoO3
Quantitative description of oxide film growth
The first physical description of the limited oxidation behavior was writ-ten by Cabrera and Mott . For very thin or ultra thin films they assume that ionic transport is the limiting growth factor. This ionic transport is caused by diffusion and affected by the electric field of the so called Mott capacitor. This Mott capacitor is created by electrons tunneling through the oxide layer to oxygen on the surface, which has empty states below the metal’s Fermi level. In the case of a constant electric potential of the Mott capacitor this model leads to the following rate equation for oxide growth :
Where uis the diffusion velocity andX1 is a characteristic length. The
diffusion velocity is given by u = u0e(W/kbT), where W is the potential
energy of a diffusion location inside the film andX1depends on the shape
of the oxide barrier, the electric potential of the Mott capacitor and the temperature.
Equation (2.1) is a differential equation which is solved by Cabrera and Mott. For thin films they knew X1 X, so they aproximated equation
(2.1) to create their inverse-logarithmic law
X = A−Blnt (2.2)
equation should be
whereτis an offset needed because the Cabrera Mott Theory is invalid
as long as there is not yet a full layer formed yet. We can rewrite this equation into
X1 X =ln
eX1/X = X
X1/X = X1
This equation can be solved, but not analytically. It requires the Lam-bert W function W(x), which is the inverse function of x = f(y) = yey. This function is in general complex and multivalued, but for x > 0 it has only one real-valued branch, W0(x). Since we are only interested in real
results we use that branch. So equation (2.8) gives
X= X1 2W0
Note that in both equation (2.2) and (2.10)dX/dt > 0 for all t, so ac-cording to this model, the film should never stop growing. Cabrera and Mott acknowledge this, but they do not provide a solution or an expla-nation. They just assume that when film thickness increases with less than 10−6 nm/s, the thickness increases so little that we can assume it has stopped increasing.
2.2 Qualitative description of oxide film growth 7
Qualitative description of oxide film growth
While the Cabrera-Mott theory gives a good quantitative description, it does not give a good qualitative description. Even worse, we know some assumptions made in the theory are wrong. At the start the theory as-sumes that there is atomic oxygen on the surface, but there is no explana-tion how it arrived there. Since atomic oxygen gas is extremely rare and thermodynamically unstable, we assume that it deposited on the surface by some oxygen containing gas. Cabrera and Mott do not address that nor ask the question what influence the type of oxygen containing gas has on the film growth. Additionally it is not taken into account that the oxide film is made out of atoms, which means that the film can only have a dis-crete thickness and it might not grow uniformly. These considerations are taken into account by Baran et al  who have investigated the oxidation of Al(111).
It all starts at the clean metal surface, which is NiAl(110) in our case. When molecular oxygen is introduced to the metal the oxygen quickly reacts with the metal surface and creates a film one monolayer thick. This layer acts as a barrier for the oxygen molecules that arrives later.
The molecular oxygen that arrives after the first layer is formed is at-tached to the newly formed oxide surface by partial dissociative adsorp-tion, as shown in figure 2.1. The oxygen molecule breaks up one of its molecular bonds and bonds to one or more aluminum atoms in the oxide. This costs energy, which is provided by electrons tunneling from the metal surface to oxygen. When the electrons are captured by the oxygen they enter a lower energy state and thus release energy. How much energy is released depends on the atom and the chemical composition, this is called the electron affinity. The net change in energy is called the adsorption en-ergy, and needs to be negative to make the reaction thermodynamically favorable.
The electrons which are tunneling through the film create a second ef-fect, which was already described by Cabrera and Mott. They create a negative charge conjugation at the surface and a positive charge conjuga-tion at the interface. This Mott capacitor creates an electric field inside the oxide, which enhances the diffusion of ions through the film.
Figure 2.1:The Mott capacitor is created electrons are tunneling through the film to be captured by the oxygen. The energy released by this process allows the molecular oxygen to partially dissociate and bond to the oxide.
face, there would be extra atoms between the support and the film, which cause lattice strain and bulging in the film. If the film grows at the surface, we expect many small islands to be formed, which will have merged into larger ones after annealing. The first option will create a curved surface without steps, while the second option creates many steps. Cabrera and Mott assumed the second option was true, but they did not give any con-clusive evidence for it. This is copied by many others, but so far we have not yet seen any conclusive experimental evidence by anybody.
The thicker the film is, the wider the tunnel barrier, and the lower the tunnel current. This decreases the charge conjugation on both the surface and the interface and thus the electric field of the Mott capacitor. This low-ers the electric force on the ions, which lowlow-ers the diffusion speed, which lowers the film growth according to Cabrera and Mott’s assumption. It does not stop it, though. The fact that the film completely stops grow-ing is due to a second effect . The lower tunnel current decreases the amount of electrons that are captured by the oxygen. Because the elec-tron affinity is fixed, less captured elecelec-trons means less energy available for oxygen dissociation, increasing the adsorption energy. When the tun-nel current becomes too low, the adsorption energy becomes positive and adsorption is no longer thermodynamically favored. The exact thickness at which this happens depends not only at the oxidizer’s electron affinity, but also on the gas pressure . That is because the Gibbs free energy
2.2 Qualitative description of oxide film growth 9
Figure 2.2: The two diffusion methods: Either the aluminum ions move towards the surface (as seen on the left) or the oxygen ions move towards the film-metal interface (as seen on the right).
pends on that gas pressure. When the oxygen is adsorbed at the surface a part of that energy is released, lowering the adsorption energy.
For alumina films on NiAl(110) in 10−6 mbar molecular oxygen the thickness limit is 2 monolayers . As we have seen in section 1, that is not enough to keep the MoO3oxidized in high pressure conditions. So we
need to increase the thickness past the 2 monolayers limit, since thicker films decrease the ion diffusion through the film and therefore reduce the speed of the reaction. Since thickness limit only depends on the adsorption energy, we know we have to either increase the gas pressure, increase the temperature, switch to an oxidizer with either a higher electron affinity or a lower bond dissociation energy . Increasing the gas pressure is easily possible, but only effective at lower pressures, since the pressure effect is mostly caused by having empty surface sites which do not exist at higher pressures. When we increase the temperature we lose the crystallinity of the film .This leaves us with changing the oxidizer. We have chosen NO2, because its electron affinity is five times higher, while its bond
All the experiments discussed in this thesis were performed at the Sputnik setup in the Kamerlingh-Onnes laboratory. This setup, consists of three linked UHV vacuum chambers, an XPS chamber in the front, a preparation and LEED chamber in the center and an STM chamber in the rear . The 3 vacuum chambers can be sealed off from each other, which allows us to only expose the center chamber to the oxygen, keeping the other chambers at 10−9 to 10−10 mbar. This not only allows us to more strictly control the oxidation of the sample, but it also prevents interference from the degassing oxygen and NO2during the measurements.
To investigate our sample we used the XPS, LEED and STM on this machine. XPS or X-ray Photoelectron Spectroscopy allows us to deter-mine the chemical composition of the top part of our sample by targeting the sample with a monochromatic 1487 eV X-ray beam. This produces electrons via the photoelectric effect, which are measured by a detector. Most electrons from the bottom of the sample are attenuated by the atoms above, so only the signal depends heavily on the composition of the sur-face. This allowed us to measure the thickness of the film as shown in section 3.5.
12 Experimental Methods
film or adsorbate is placed on the surface of the sample the interference pattern will produce extra spots which match the atomic structure of the film. This gives us information about the surface as a whole, allowing us to see whether the film is well-structured or not and whether its crystal structure has changed.
Scanning Tunneling Microscopy or STM is the third technique we used. STM setups consist of a single atom movable tip close to the sample sur-face. When a voltage is applied between the conducting sample and the tip a small tunneling current will be created. The magnitude of that cur-rent depends on the distance between the tip and the conducting part of the sample. So a feedback loop can be created to keep the tip on a fixed height above the sample while scanning the sample horizontally. That way we create a height map of the conductive surface up to atomic level. Be-cause alumina insulates we cannot detect the film directly with STM. We can however measure the height of the NiAl underneath it. That means that we can get a good view of the Alumina-NiAl interface. This allows us to answer one of our main questions: where does the alumina film grow. Growth at the interface should be visible, growth at the surface should not.
For our main experiment we first need a crystalline oxide film. First the metal surface is cleaned as described in section 3.3, after which it is oxi-dized with O2 to the saturation point. This surface is thoroughly
inves-tigated with Low Energy Electron Diffraction, Scanning Tunneling Mi-croscopy and X-ray Photoelectron Spectroscopy. All LEED patterns were imaged with an electron energy of 67 eV, and for the thorough XPS mea-surement we measured the Al2p, Ni3p, O1s, C1s and N1s peaks. If the oxide film surface is clean we can start the experiment. The surface is subsequently oxidized by NO2 and annealed. Every two NO2 oxidation
cycles the surface has been investigated with LEED and XPS, measuring Al2p, Ni3p and O1s. After 8 and after 20 cycles we also took a more thor-ough XPS measurement and a STM measurement.
After 20 cycles, it was just barely possible to scan the surface with well enough resolution. Since the quality of the STM images would further de-crease if we would make the film thicker, we decided to not inde-crease the film any further. On the thick alumina film molybdenum oxide nanoparti-cles were deposited by evaporating molybdenum metal in an atmosphere of molecular oxygen at room temperature. Directly after an XPS spectrum is measured to see whether the particles are stable or not. In section 1 we
3.3 Sample preparation 13
have seen that they are unstable on a 5.35 ˚Afilm, the results for the thicker films can be found in section 4.4.
For the second, smaller experiment we did the following: We started with a clean alumina film surface cleaned and oxidized with O2 as
de-scribed in 3.3. The surface is dosed with 5×10−7NO2for 5 minutes at 650
K, a 10 times higher pressure than we do for the main experiment, and in-vestigated by STM. After this the sample is annealed for 7 minutes at 1120 K and given a second dose of No2, by dosing it with 5×10−7 NO2 for 5
minutes at 650 K and annealing 7 minutes at 1120 K. After this it is investi-gated by STM again. Doing so we can see better at which location the film is growing. The STM data gathered here is therefore used in section 4.3, where we discuss the results.
Our cleaning method has been based on Song and Yoshitake’s paper on cleaning NiAl(110):
• Once sputter for 25 minutes at 1.5 keV with 4×10−7 mbar Ar, fol-lowed by annealing for 50 minutes at 1300 K, and cooling down to 570 K.
• Once sputter for 15 minutes at 1.5 keV with 4×10−7 mbar Ar, fol-lowed by dosing 1×10−6mbar O2for 5 minutes at 1300 K annealing
for 25 minutes at 1300 K, and cooling down to 570 K. If there was a high carbon signal in the last XPS measurement, this is repeated once or twice more.
• Twice sputter for 15 minutes at 1.5 keV with 4×10−7 mbar Ar, fol-lowed by annealing for 30 minutes at 1300 K, and cooling down to 570 K.
• Three times sputter for 15 minutes at 1.5 keV with 4×10−7mbar Ar, followed by annealing for 25 minutes at 1300 K, and cooling down to 570 K.
The crystal was oxidized using O2 with the following method, which
has been shown to create a crystalline oxide :
• Once dose 5×10−6 mbar O2 for 5 minutes at 570 K, increase the
14 Experimental Methods
• Once dose 5×10−6 mbar O2 for 10 minutes at 570 K and anneal 5
minutes at 1120 K.
• Once dose 1×10−6 mbar O2 for 10 minutes at 570 K and anneal 5
minutes at 1060 K.
Oxidation cycles using NO2consist of dosing 5×10−8NO2for 5
min-utes at 650 K, after which the sample is annealed for 7 minmin-utes at 1120 K.
The higher oxidation temperatures are necessary if we want the film to grow to its Cabrera Mott limit. If the temperature is too low, the alumina atoms used to create the film can not be replaced fast enough, and a pure nickel layer can be formed. Such a layer will stop the film growth, before its limit is reached. Cai et al  have shown that at 298 K the nickel layer is formed, but at 573 K it is not. So based on that we oxidize our film at 570 K.
Figure 3.1:NiAl XPS signal after 20 cycles (6000 s) of NO2oxidation. To improve
readability the two peaks of each doublet aren’t displayed separately, but only their combined contribution. The four peaks from left to right are Al2p surface, Al2p interface, Al2p bulk and Ni2p bulk.
3.4 XPS Fitting 15
The XPS data is fitted using CasaXPS. All 13 measurements are fitted with the same boundary conditions: The NiAl region was fitted with 4 doublet peaks: Ni3p, Al2p bulk, Al2p interface and Al2p surface. The doublet peaks are fitted with two Gaussian-Lorentzian peaks with the same full With half Maximum. The area of the high energy peak was fixed to half of the low energy peak, since the split is due to spin-orbit coupling. For the Al2p peaks we have used the energy split used by Sharovsky et al , which is 0.5 eV. For the Ni3p peak no good split value could be found, so that parameter is left free.
Figure 3.2:Oxygen XPS signal after 20 cycles (6000 s) of NO2oxidation.
16 Experimental Methods
the film thickness measurement.
XPS measurement of film thickness
According to Seah and Spencer, the attenuation AABof the photoelec-trons from a deeper layerBthrough layer Ais given by
WheredA is the thickness of layer A, λAB is the attenuation length of the photoelectrons from layerBthrough layerAand cosθis the angle between
the surface normal and the detection angle. That angle is always 90◦in our case. The attenuation length is given by 
(ZA)0.45ln(EB/27) +3 +4
Where NA is the atomic density of A, EB is the kinetic energy of the pho-toelectrons fromBandZAis the average atomic number of layerA.
The production of photoelectrons in a thin layer is given by
IA = IA∞(1−AAA) = IA∞
Our sample consists of a NiAl bulk support, followed by a AlOx inter-face and and one or two AlOy surface layers. Using the equations above that leads to:
Is = Is∞(1−Ass) = Is∞
Ii = Ii∞(1−Aii)Asi = Ii∞
di λii exp ds λsi (3.5)
Ib = Ib∞AibAsb = Ib∞exp
di λib exp ds λsb (3.6)
wheresis the surface layer,ithe interface layer andbthe bulk support. In most XPS thickness calculations, one would now derive ds from a combination of these equations. In such a case one assumes that the film homogeneously thick across the sample. For thicker films that assumption is valid, the film grows faster at thinner parts, so this self-correcting effect
3.5 XPS measurement of film thickness 17
will create a film of homogeneous thickness. But when a film is only 2 or 3 layers thick, as it is in our case, even the smallest change gives a 50% increase, which renders this assumption invalid.
Being unable to use this standard approach, we decided to make our own model. From the theory we know that it is much harder to grow oxide on a 3 layer film than it is on a 2 layer film. When we anneal enough we will only grow one layer at the time. This allows us to create a two level model, where α is the part of surface covered with 3 layers, and 1−α is
the part covered with 2 layers. Using that gives
Is =αIs3l+ (1−α)Is2l =
Is∞α(1−A2ss) +Is∞(1−α)(1−Ass) =
Ii =αIi3l+ (1−α)Ii2l =
λii α exp
Ib =αIb3l+ (1−α)Ib2l =
Ib∞Aib(αAsb2 + (1−α)Asb)
With the average film thickness being
davg =d3lα+d2l(1−α) =
(2ds+di)α+ (ds+di)(1−α) = (ds+di) +dsα (3.10)
To get the average thickness we need to solve (3.7), (3.8) and (3.9) forα. The
easiest way to do so is by taking the Al2p peaks, since the bulk, interface and surface are three different peaks there. However, as we have shown in section 3.4 it is hard to get the fitting for the surface and interface peaks right, since they overlap so much. We therefore decided to use the O1s peaks.
18 Experimental Methods
thickness calculation, like we could for the Al2p peaks. We need to use their sumIt and extract the surface and interface signals from there.
ss−(1−α)Ass] + IIbi∞∞(1−Aii)[αA2si+ (1−α)Asi]
Aib[αA2sb+ (1−α)Asb] =
[1−αA2ss−(1−α)Ass] + Ii∞
(1−Aii)[αAsi2 + (1−α)Asi]
Since we want to solve this equation forαwe move them all to one side to
sb−Asb) + Is∞
This formula can be used directly if Ib∞, Is∞ and Ii∞ are known. In the case of thin films this is impossible, since the thick films have a different crystal structure, and therefore a different I∞. We can however calculate the ratios between the different intensities :
WhereN0is the atomic density of the element,σis the photoionization
cross section, which is a sensitivity factor,λis the attenuation length, and
T is the transmission function. Note that this N0 is different than the N
from equation 3.2. In that equation the total number of atoms per unit
3.5 XPS measurement of film thickness 19
volume is used, while here we only count the atoms of the element whose signal we measure.
ss−Ass)− N 0
si−Asi) (3.16) Since the interface layer and surface layer signal are at the same energy,
σi =σs =σt,λii =λss =λttand Ti =Ts =Tt.
s(1−Ass) +Ni0(1−Aii)Asi It
sb−Asb) +Ns0(A2ss−Ass)−Ni0(1−Aii)(A2si−Asi) =
bAibAsb+Ns0(1−Ass) +Ni0(1−Aii)Asi It0
bAib(A2sb−Asb) +Ns0(A2ss−Ass)−Ni0(1−Aii)(A2si−Asi) (3.17)
where IA0 = IA
σAλAATA is the corrected intensity. Our XPS software
al-ready calculates IA
λAATA, so if we want to calculate the corrected intensity
we only need to knowσA. Getting the right value forσAis hard. There are big discrepancies between experimental and theoretical data, and experi-mental data is in general only available for the main peak of each element. For the Nickel 2p peak, for example, we could not find any convincing data. Therefore we decided to use them as a fitting parameter.
We know that our substrate is 50% nickel and 50% aluminum, soNNi =
NAl. So the corrected intensity on a sample without film should be the same. So the corrected intensity ratio of a sample with film would simply be the ratio of the attenuation. For a two layer film that means
INi0 IAl0 =
And for a three layer film we get
INi0 IAl0 =
20 Experimental Methods
at different thicknesses to average out the fitting errors. We can now use the definition of the corrected intensity to calculate the sensitivity factor
σAl = I
Because the sensitivity factor depends mostly on the atomic number, we assumed thatσAlis the same for all aluminum species we have. ForσO we used the fact thatα = 0 when we only dosed with O2. Since only the
numerator can makeαzero, this gives
(1−Ass) + Ii∞
Putting in equation 3.15 and rearranging gives
(1−Ass) + Ni
Nb(1−Af f) +
With the equations for the sensitivity factor we can calculate the cor-rected intensity I0A = IA
σAλAATA, which is the last quantity we needed to
know in order to calculate the thickness using equation 3.17.
Results and discussion
Figure 4.1: LEED patterns of our surface, with a) 0 s of NO2 oxidation, b) 2400 s
of NO2oxidation, c) 4800 s of NO2oxidation and d) 6000 s of NO2oxidation.
22 Results and discussion
have made a LEED measurement, and the results can be found in figure 4.1.When looking at those patterns the first thing we see is that there is very little change in the unit cell of the film. After 6000 s the unit cell is the same as the one we started with. Since we know that the unit cell did not change, we now also know that all unit cell related properties did not change, and that many literature sources are still valid, even for higher thicknesses. Comparing the LEED patterns with literature  does not show big changes either, which gives further evidence that we have cre-ated a crystalline film which remained crystalline when it becomes thicker. When the sample is placed in the STM we can directly image the unit cell and compare it with said literature. On the top of the image there are clear rows about 1.5 to 2.0 nm wide. From Simon et al  we know the unit cell of the top oxide layer is 1.7 nm wide, so that fits well with our estimation.
Figure 4.2:STM image showing the size of the unit cell of our alumina film, which is between 1.5 nm and 2.0 nm wide. The image is 80 nm x 80 nm and taken in UHV conditions, with -1 V bias voltage and 100 pA tunneling current.
When combining the results from the STM and the LEED with the cited literature sources, it is easy to conclude that our film has the same unit cell that has been reported numerous times for alumina on NiAl(110). Still unknown is the question whether or not the structure inside the unit cell changed. We simply did not have the STM resolution to either confirm or
4.2 Film thickness 23
reject that. But one could say that it would be very remarkable to have a change in crystal structure without a change in unit cell. Therefore we think it is save to say that the crystal structure did not change much, and that all the crystal structure related properties, did not change much either.
One of the main questions we wanted to answer asks about the increase of the oxide thickness due to the NO2 oxidation. With the XPS data and
equation (3.17) we can now calculate the thicknesses, which are shown in figure 4.3.
Figure 4.3: The film thickness measurement, with equation (2.10)fitted with pa-rametersX1 = 62.9A,˚ u = 1.68×104 A/s and˚ τ = 241s. The point (0,5.35) is
fixed as is done before in section 3.5, since that point is very well known from literature.
24 Results and discussion
of the peaks of the XPS spectrum. All literature says that extra NO2 will
increase the thickness of the film, or if the limit is reached stagnate the growth. To see whether or not that is true we would have to calculate the size of the measurement error. Unfortunately that is not possible. Not only does our fitting program not give any error information, there is also no direct fitting method. One has to assume the exact energy of the peaks and although they are generally known from literature, Popova et al  have shown that the the energy can increase or decrease based on film thickness. Beside this we also have the problem that the interface peak can not be resolved which shows that we have too little energy resolution to properly fit the peaks of this system.
This doesn’t mean we can’t learn anything from this data. One of the main achievements of the Cabrera Mott theory was the prediction of the film growth. Since we now have film growth data we wanted to test this prediction, by fitting our data in figure 4.3 to equation (2.10):
X= X1 2W0
Cabrera and Mott have given a range for the values of X1 and u .
They say thatX1should be between 100 ˚Aand 1000 ˚A. This is larger than we have measured, but the error is less than an order of magnitude. Know-ing the error margins in our data their range might very well be right. For
uthey do not give a fixed range, they only say thatu=u0exp(−W/kbT), where W is the potential energy of an diffusion location inside the film and u0 ∼ 1012 A/s or less. No information is available on˚ W, so it is im-possible to calculate u0 for our case. The offset τ has been proposed by
Ghez’s adjustments to the original theory . In his paper he eventually assumes τ to be very small and thus can be ignored, which works well
for the cases he studies. In our caseτ = 241 s, which is big enough that
it cannot be ignored. The reason for this lies in the method discussed in section 3.2. We first create a full 5.35 ˚Athick oxide film with O2, before
starting our NO2 experiment. Therefore our timing is different from the
case where one would start directly with NO2, so it expected thatτ could
not be ignored.
Another remark has to be made with regards to the qualitative work of Baran et al  which is explained in section 2.2. They show why there is a limit, but don’t give an equation for that limit if the exact reaction process is unknown, like it is for NO2. Even in the cases they have studied
them-selves, they don’t give an estimate on the thickness at which the Cabrera Mott theory starts to fail. Judging our own data does not give such a value
4.3 Film growth location 25
either. At 5400 s the fit fits perfectly to the data. One really needs to oxidize for a longer period or at a higher pressure in order to get such information.
Film growth location
Like we have explained in section 2.2 it is still unknown whether the alumina film grows at the surface or the interface. With our setup we should be able to distinguish the two. To do so a clean oxidized surface was scanned with STM, the dosed with 5×10−7 mbar NO2and scanned
again, followed by being annealed at 1130 K. After two of those cycles we scanned again. The results are in figure 4.4.
Figure 4.4: STM images of our alumina on NiAl(110) sample before NO2
oxida-tion (top left), after oxidaoxida-tion (top right) and after annealing and a second round of oxidation and annealing (bottom). All images are 80 nm x 80 nm and taken in UHV conditions, with -1 V bias voltage and 100 pA tunneling current.
in-26 Results and discussion
crease in tiny islands, which means that those areas used to be conductive are now becoming insulating. NiAl is conductive and alumina insulating so NiAl is replaced by alumina, which means that the film grows at the interface. After annealing the small vacancy islands merge together, since that is more thermodynamically favorable and the annealing provides the thermal energy to do so.
Stability of MoO3
Figure 4.5:After depositing the MoO3the aluminum and nickel bulk peaks have
decreased, which shows that the film has grown. The alumina peak moved to a lower energy, indicating that the alumina film has changed in chemical composi-tion.
Now we know how the oxide film grows, what does and does not change, it is time to investigate the stability of MoO3 nanoparticles on
the thicker film. The average film thickness is measured before and after molybdenum oxide deposition. Before deposition the film had an aver-age thickness of 6.9 ˚A, after deposition that is raised by 0.9 ˚Ato 7.8 ˚A. One could argue that the film itself did not grow, since according to section 3.5 this measurement only uses the support and oxygen intensities. The support signal is attenuated by the molybdenum oxide nanoparticles like
4.5 Carbon contamination 27
it is by the alumina film, and both the film and the nanoparticles contain oxygen. We think this is incorrect, because of two reason. First, the alu-minum bulk peak has decreased more than the nickel peak (-12.8% for the Al bulk peak versus -10.2% for the Ni bulk peak). This indicates that the top NiAl layer got deprived of aluminum. If the film grows at low temper-atures, like we think has happened here, Cai et al  have shown that an aluminum deprived layer forms just beneath the film. Secondly, although it shifted so much in energy that our software could not fit the peak cor-rectly, it is clear that the Al3+ peak itself grew. This could not have any other cause than the increase of the film thickness.
Carbon is one of the impurities in the NiAl crystal we have been using. As long as it stays away from the surface it does not influence the exper-iments. To measure whether is does or not, we used XPS. XPS is only sensitive in the top 10 nm of the sample, which is the film and the area just beneath it. Three times we have measured the Carbon XPS-signal, at the beginning, after 2400 s of NO2oxidation and after 6000 s of NO2oxidation,
shown in figure 4.6. The results are unexpected: It looks like the first 2400 s of oxidation brought up more carbon near the surface, but the 3600 s of oxidation thereafter made it disappear.
To look for the cause we have to realize that there are two different pro-cesses at play here. One is the diffusion of the carbon through the sample. Under homogeneous conditions, the carbon atoms will diffuse and end up in a homogeneous uniform distribution. The second process is the chem-ical reaction between the surface oxygen and the bulk carbon atoms. The carbon atoms prefer to be at the surface because they can create carbon particles there. But even more energetically favorable is the creation of CO2gas. The carbon and oxygen atoms form CO2 which is then pumped
off by our system.
28 Results and discussion
Figure 4.6: XPS spectra of the C1s peak before NO2oxidation (blue), after 2400 s
of NO2oxidation (red) and after 6000 s of NO2oxidation (green).
We have investigate the stepwise NO2 oxidation of an alumina film on
NiAl which has already been oxidized with O2 up to 5.35 ˚A, finding a
thickness where MoO3nanoparticles are stable. The surface has been
in-vestigated every step with LEED, XPS and regularly STM as described in section 3.2.
Within the 11 LEED measurements performed we have seen very little change in the unit cell of the film. The LEED patterns and STM unit cell images correspond very well with the pattern and unit cell known from literature . The crystal structure could not be observed directly, but it is very unlikely that the crystal structure changed without changing the unit cell. Using this fact we have shown that Ghez’ adjustment  to the Cabrera-Mott theory , given by equation (2.10), is at least valid up to 6.9 ˚A. At that thickness the film still grew fast, as can be seen in figure 4.3. This shows that the thickness limit of NO2 oxidation, which predicted by Baran et al  as a hard limit, has not yet been reached.
Fitting of the thickness data has given us the values of the characteristic length X1 =62.9 ˚A, diffusion velocityu = 1.68×104 A/s and time offset˚
τ = 241 s. Although the errors on the data and the fit are big, they do
correspond with the estimations given in the original article .
According to our measurement, the MoO3nanoparticles are still
unsta-ble on the thicker films. We deposited them on the 6.9 ˚Athick alumina film, which was the thickest film we could still scan on. Unfortunately, as one can see in figure 4.5 the MoO3 nanoparticles were unstable and increased
the film thickness from 6.9 ˚Ato 7.8 ˚A. This all happened at low tempera-ture, and all the low temperature effects described by Cai et al  have been recorded.
cation of the oxide growth. STM images shown in figure 4.4 clearly show an increase in the number of conducting islands, which can only be ex-plained if the oxide grows at the interface and not at the surface, since the alumina film is not conduct.
 G. Kresse, M. Schmid, E. Napetschnig, M. Shishkin, L. K ¨ohler, and P. Varga, Structure of the ultrathin aluminuium oxide film on NiAl(110) solved by STM and DFT., Science1440(2005).
 N. Cabrera and N. F. Mott,Theory of the oxidation of metals, Reports on Progress in Physics12, 163 (1949).
 R. Ghez, On the Mott-Cabrera oxidation rate equation and the inverse-logarithmic law, The Journal of Chemical Physics58, 1838 (1973).  H. Freund,Formation of a well-ordered by oxidation of NiAl ( 110 ),
Sur-face and InterSur-face Analysis259, 235 (1991).
 G. H. Simon, M. Heyde, and H.-J. Freund, Imaging and manipulation of adatoms on an alumina surface by noncontact atomic force microscopy, Journal of Physics: Condensed Matter24, 84007 (2012).
 R. V. Mom, M. J. Rost, J. W. Frenken, and I. M. Groot,Tuning the Prop-erties of Molybdenum Oxide on Al2O3/NiAl(110): Metal versus Oxide De-position, Journal of Physical Chemistry C120, 19737 (2016).
 J. D. Baran, H. Gr ¨onbeck, and A. Hellman, Mechanism for limiting thickness of thin oxide films on aluminum, Physical Review Letters112, 1 (2014).
 C. Ocal, S. Ferrer, and N. Garc´ıa,Cabrera-Mott mechanism for oxidation of metals explains diffusion of metallic atoms through thin defective oxide layers, Surface Science163, 335 (1985).
 N. Cai, G. Zhou, K. M ¨uller, and D. E. Starr,Tuning the limiting thickness of a thin oxide layer on Al(111) with oxygen gas pressure, Physical Review Letters107, 1 (2011).
 T. T. Lay, M. Yoshitake, and W. Song, Epitaxial growth of well-ordered ultra-thin Al2O3 film on NiAl (1 1 0) by a single-step oxidation, Applied Surface Science239, 451 (2005).
 K. M. Ervin, J. Ho, and W. C. Lineberger,Ultraviolet photoelectron spec-trum of nitrite anion, The Journal of Physical Chemistry92, 5405 (1988).  M. J. Travers, D. C. Cowles, and G. Ellison,Reinvestigation of the elec-tron affinities of O2 and NO, Chemical Physics Letters164, 449 (1989).  C. T. Herbschleb, P. C. Van Der Tuijn, S. B. Roobol, V. Navarro, J. W.
Bakker, Q. Liu, D. Stoltz, M. E. Ca ˜nas-Ventura, G. Verdoes, M. A. Van Spronsen, M. Bergman, L. Crama, I. Taminiau, A. Ofitserov, G. J. C. Van Baarle, and J. W. M. Frenken,The ReactorSTM: Atomically resolved scanning tunneling microscopy under high-pressure, high-temperature cat-alytic reaction conditions, Review of Scientific Instruments 85, 083703 (2014).
 W. Song and M. Yoshitake, Effects of surface cleaning on oxidation of NiAl(110), Applied Surface Science241, 164 (2005).
 M. Jaeger, H. Kuhlenbeck, J. Freund, M. Wuttig, W. Hoffmann, R. Franchy, and H. Ibach, Formation of a well-ordered by oxidation of NiAl(110), Surface Science259, 235 (1991).
 N. Cai, H. Qin, X. Tong, and G. Zhou, Growth of ultrathin amorphous alumina films during the oxidation of NiAl(100), Surface Science618, 20 (2013).
 A. Shavorskiy, K. M ¨uller, J. T. Newberg, D. E. Starr, and H. Bluhm,
Hydroxylation of Ultrathin Al 2 O 3 /NiAl(110) Films at Environmental Humidity, The Journal of Physical Chemistry C118, 29340 (2014).  N. M. Martin, J. Knudsen, S. Blomberg, J. Gustafson, J. N. Andersen,
and E. Lundgren,High-resolution core-level spectroscopy study of the ul-trathin aluminum oxide film on NiAl ( 110 ), Physical Review B125417, 1 (2011).
 M. P. Seah and S. J. Spencer, Ultrathin SiO2 on Si IV. Intensity mea-surement in XPS and deduced thickness linearity, Surface and Interface Analysis35, 515 (2003).
 P. J. Cumpson and M. P. Seah, Elastic Scattering Corrections in AES and XPS. II. Estimating Attenuation Lengths and Conditions Required for their Valid Use in Overlayer/Substrate Experiments, Surface and Inter-face Analysis25, 430 (1997).
 S. Hofmann, Auger- and X-Ray Photoelectron Spectroscopy in Materi-als Science, volume 49 ofSpringer Series in Surface Sciences, Springer, Berlin Heidelberg, 1 edition, 2013.
 J. Libuda, F. Winkelmann, M. B¨aumer, H. J. Freund, T. Bertrams, H. Neddermeyer, and K. M ¨uller,Structure and defects of an ordered alu-mina film on NiAl(110), Surface Science318, 61 (1994).